Introduction • ancient constructions were built using mud walls reinforced with woven bamboo mats, reeds or straw (mud+straw =Adobe). • In the present form, the FERROCEMENT may be defined as a composite material obtained by reinforcing the cement mortar with steel fibers in the form of a wire mesh as shown in Figure 8.1.
While the mortar provides the mass, steel fiber imparts tensile strength and ductility to the material. • More accurately, FERROCEMENT may be considered as a special form of reinforced concrete construction with more closely layered wire meshes than a material of construction. • Due to the distribution of a small diameter wire mesh reinforcement over the entire surface, and sometimes over the entire volume of the matrix, a very high resistance to cracking is obtained. • Also, toughness, fatigue resistance, impermeabilty etc. are considerably improved.
Mixture of Ferrocement • The FC composite is a rich cement-mortar matrix of 10 mm to 60 mm thickness with a volume reinforcement consisting of either welded mesh or mild steel bars.
The matrix is typically rich in cement, i.e. a cement-sand ratio of 1:1.5 or 1:2 is used. • Portland cement, with or without pozzolana, is generally used for FC. • Plasticizers and other admixtures may also be added to improve the workability. • Therefore, sands with maximum sizes of 2.36 mm and 1.18 mm are recommended for FC mixes. • A water/cement ratio of 0.3 to 0.4 is recommended.
Reinforcement For Ferrocement • Skeleton Steel Frame: It is made confirming exactly to the geometry and shape of the structure. It comprises relatively large diameter (about 3 to 8 mm) steel rods spaced typically 70 to 100 mm. It may be tied reinforcement or welded wire fabric. • Wiremesh: Consists of galvanized wire of diameter 0.5 to 1.5 mm spaced at 6 to 20 mm center-to-center, is formed by welding or twisting. • The required number of layers of wire mesh are fixed on both sides of the skeleton frame. • A spacing of at least 1 to 3 mm is left between two mesh layers. Wherever two pieces of the mesh are joined, a minimum overlap of 80 mm should be provided and tied at a close interval of 80 to 100 mm center-to-center.
Placing of FC (Impregnation of Meshes With Matrix) • This is the most critical operation in ferrocement casting. • Sufficient quantity of mortar is impregnated through mesh layers so that the mortar riches the other side and there are no voids left in the surface. • A wooden hammer of about 100 mm diameter with 150 mm long wooden handle can be used for hammering over the temporarily held form. • This will give sufficient vibrations for compacting the mortar. As soon as it is ensured that the mortar penetration through the mesh is satisfactory, the form is shifted to the next position. • In structures where many layers are used as reinforcement and the thickness is more than 20 cm, it is advisable to do the casting in 3 layers.
Corrosion Protection • For normal applications, the mortar provides adequate protection against corrosion of reinforcement, but where the structure is subjected to chemical attack by the environment as in sea water, it is necessary to apply suitable protective coatings on the exposed surface. • Venyl and epoxy coatings have been found to be especially satisfactory on structures exposed to sea water and also in most other corrosive environments. • For protection against a less severe environment, cheaper asphaltic and bituminous coatings are generally satisfactory.
Properties Of Ferrocement • The load carrying capacity of FC is correlated with the specific surface area of reinforcement : Specific Surface Area= Awire / Vcomposite • Ferrocement has tensile strength as high as its compressive strength i.e. 27 MPa, and the widths of cracks are very small even at failure (about 0.05 mm). • FC structures can be designed to be watertight at service loads. • Impact tests on FC slabs show that damage due to impact reduces with increasing specific surface and ultimate strength of mesh. • Fatigue tests on FC beams show poor resistance of FC under cyclic loading.
Applications • FC is a popular structural composite to manufacture many precast products, such as watertanks, silos and bins, pipes, shell roofs, floor units, wind tunnel, permanent forms of concrete columns. The major advantages are as follows; • FC structures are thin and light. • 30% reduction in dead weight on supporting structure, 15% saving in steel consumption and 10% in roof cost has been estimated. • suitable for manufacturing the precast units which can be easily transported. • The construction technique is simple and does not require highly skilled labour. • Partial or complete elimination of formwork is possible. • FC construction can be easily repaired in case of local damage due to abnormal loads.